Certificate of Analysis
First Issued: 1994
Version: August 1997
WGB-1 was obtained from the Wellgreen Complex, Yukon Territory, Canada. WGB-1 was prepared and certified in cooperation with the Analytical Method Development Section of the Mineral Deposits Division of the Geological Survey of Canada (GSC).
The mineralogy of this gabbro rock consists of plagioclase feldspar, pyroxene, chlorite, prehnite and calcite. Sulphide mineralization in the sample is sparse and includes chalcopyrite, pyrrhotite, pentlandite and galena (intimately associated with the pyrrhotite). Other minerals identified include titanite, ilmenite and rutile.
WGB-1 is intended for analysis of platinum-group elements in exploration samples and for other samples where very low concentrations of gold and PGEs are required. WGB-1 is also intended for general rock analysis for a gabbro-type rock.
INSTRUCTIONS FOR USE
WGB-1 should be used "as is" without drying.
METHOD OF PREPARATION
The rock was hand-picked by a GSC geologist. The raw material was dried, comminuted and sieved to obtain a -74micron (-200 mesh) product which was blended and bottled.
The homogeneity of the stock with respect to its gold, platinum and palladium contents was confirmed using bottles chosen according to a stratified random sampling scheme. The analytical method was a fire-assay preconcentration followed by an inductively-coupled plasma – mass spectrometric (ICP-MS) finish performed at GSC. The homogeneity was also confirmed, at a commercial laboratory, for all major constituents by X-ray fluorescence.
WGB-1 was certified by an interlaboratory analysis program. Thirty-three university, commercial, and government laboratories from Canada, United States, Europe, Australia, Africa, and Japan participated in an interlaboratory certification program. Up to 80 elements were analyzed by methods of each laboratory's choice. A statistical analysis of the data yielded certified values for gold, palladium, platinum, Fe2O3, K2O, MgO, and chromium. Provisional values were assigned for rhodium, iridium and thirty-two others. Informational values for ruthenium and other elements are also given.
The Canadian Certified Reference Materials Project has prepared this reference material and statistically evaluated the analytical data of the interlaboratory certification program to the best of its ability. The purchaser, by receipt hereof, releases and indemnifies the Canadian Certified Reference Materials Project from and against all liability and costs arising out of the use of this material and information.
Further information is available upon request to:
CCRMP, CANMET-MMSL (NRCan)
555 Booth Street, Ottawa
Telephone: (613) 995-4738
Facsimile: (613) 943-0573
|Certified Constituents||Au, ng/g||Pd, ng/g||Pt, ng/g|
|95% Conf. Limits||± 1.1||± 2.1||± 1.6|
|Certified Constituents||Fe2O3 %||K2O %||MgO %||Cr, µg/g|
|95% Conf. Limits||± 0.14||± 0.04||± 0.19||± 13|
|Provisional Constituents||Ir, ng/g||Rh, ng/g||Ru, ng/g|
* Informational value
|Provisional Constituents||Mean||95% Conf, Limits||Provisional Constituents||Mean||95% Conf, Limits|
|Al2O3 %||11.15||± 0.27||Nb, µg/g||8||± 4|
|CaO, %||15.78||± 0.85||Nd, µg/g||9.9||± 0.9|
|MnO, %||0.143||± 0.014||Ni, µg/g||76||± 7|
|Na2O, %||2.15||± 0.08||Rb, µg/g||19.5||± 1.5|
|P2O5, %||0.099||± 0.034||Sb, µg/g||2.0||± 0.4|
|SiO2, %||49.1||± 0.8||Sc, µg/g||44||± 4|
|TiO2, %||0.84||± 0.07||Sm, µg/g||2.8||± 0.3|
|Ba, µg/g||851||± 61||Sr, µg/g||118||± 9|
|Co, µg/g||29.8||± 1.7||Tb, µg/g||0.5||± 0.1|
|Cs, µg/g||0.52||± 0.15||Th, µg/g||1.0||± 0.1|
|Cu, µg/g||106||± 9||U, µg/g||0.75||± 0.1|
|Eu, µg/g||1.27||± 0.06||V, µg/g||222||± 17|
|Hf, µg/g||1.5||± 0.2||Y, µg/g||14.6||± 2.7|
|Ho, µg/g||0.52||± 0.07||Yb, µg/g||1.42||± 0.18|
|La, µg/g||8.7||± 1.1||Zn, µg/g||31.5||± 8.5|
|Mo, µg/g||1.2||± 0.5||Zr, µg/g||44||± 16|
|Informational Ranges||Informational Ranges|
|H2O %||0.16 - 0.21||Gd, µg/g||2.5 - 3.5|
|LOI %||3.6 - 4.0||Ge, µg/g||0.2 - 7|
|S total %||0.01 - 0.03||Hg, µg/g||0.01|
|Ag, µg/g||0.1 - 1||Li, µg/g||43 - 51|
|As, µg/g||1.5 - 5||Lu, µg/g||0.20 - 0.36|
|B, µg/g||250 - 280||Pb, µg/g||4 - 14|
|Be, µg/g||0.2 - 0.8||Pr, µg/g||2.3 - 2.6|
|Bi, µg/g||0.1 - 2||Se, µg/g||0.1 - 0.8|
|Cd, µg/g||0.1 - 0.4||Sn, µg/g||4.2 - 5.2|
|Ce, µg/g||14 - 20||Ta, µg/g||0.3 - 1|
|Dy, µg/g||2.5 - 3.5||Th, µg/g||1.0 - 1.6|
|Er, µg/g||1.2. - 1.8||Tm, µg/g||0.15 - 0.30|
|Ga, µg/g||11 - 13||W, µg/g||1 - 3.5|
- Date Modified: